The microstructure of the SLM parts strongly influences their physical and mechanical properties. The examination of the microstructure can help understand the effect of the laser beam on the powder bed and the melting pool behaviour during the SLM build.
To examine the microstructure of the SLM parts under Nikon Optiphot optical microscope and LEO 440 SEM, the samples were cut, polished and etched based on the practice standard ASTM E407. Thin wall samples were selected for checking the phase, grain size and grain growth direction under single laser moving track on each layer. Since the laser tracks started and ended in the same position and moved in the same direction on each layer for building thin wall in SLM process, it was possible to examine a whole layer in one horizontal view. Also choosing thin walls rather than cubic blocks allowed clear details discovered in both horizontal and vertical directions by removing the scan overlap effect.
FEI Nova 600 Nanolab Dual Beam EBSD used in powder sustainability study was also used to investigate the phase, grain size and grain growth direction of the SLM thin wall parts. It detected the crystallographic orientation which can be used on phase identification, and also showed clear grain boundaries.
The information given by EBSD can be a supplement to optical microscopy and SEM examination.
Experiments were carried out to gain better understanding on the main factors which affect the SLM process. This knowledge helps to optimise the SLM manufacturing process and control the final part’s quality.
Firstly, the equipment controllable SLM processing parameters were investigated. The optical scanning system was examined to find the
relationship between the input laser energy density and the manufactured part’s physical and mechanical properties. Then different process scanning strategies were studied and their effects on the manufactured part’s quality were investigated experimentally. Building conditions were studied to gain the knowledge of their influence on the melting process.
After studying the main SLM process parameters, an experimental programme continued to investigate the raw material’s effect on SLM build quality. As base materials used in the manufacture process, the powders’
performance when they are spread and placed on the laser processing area can impact the laser melting process and the final part’s quality. The powder’s particle shape and size distribution, powder bed density, powder flowability and sustainability were investigated for their effect on SLM parts quality.
Material properties needed in the simulation work, especially the density and thermal properties of the powder bed were experimentally measured for use in the heat transfer model. Particular measurement experiments were designed and relevant calculations were used to obtain reliable values.
Finally, the microstructure of the built parts was examined experimentally by optical microscope, SEM and EBSD. Results obtained in this experiment process gave better understanding of the laser melting process, and also were used to validate the prediction from the heat transfer model.
These experiments enable to understand the key factors which affect the SLM process and final parts quality. This helps to obtain an idea on which process parameter needs to be considered and involved in the modelling work. The experimental programmes also provide the correct model inputs for a reliable and accurate simulation, as well as the validation for the prediction from the heat transfer model. These are the main contributions to this research.
78 4 Finite Element Modelling Methods
The effect of the main SLM processing parameters on the manufactured part’s quality can be investigated from experiments. By controlling these parameters, the whole SLM process can be optimised. However, key factors which describe and determine the melting process such as the melting pool behaviour and thermal history on the powder bed are not easy to be measured and investigated from an experimental programme. A reliable analysis model can simulate the melting process, predict essential behaviours during the manufacturing, and therefore give in-depth knowledge of the SLM process for better control. This chapter describes the methods to establish a heat transfer analysis model for simulating the laser melting process and predicting the temperature distribution and part’s microstructure in the SLM process.
Compared with analytical models, finite element model establishment requires more efforts on the inputs and model structure study, and can provide accurate and detailed results for further analysis. The heat transfer model in the study was established in ABAQUS/CAE v6.9-6.11 which is a software application used for both the modelling and analysis of mechanical components and visualizing the finite element analysis result. It was developed and released by Dassault Systèmes as a main component of brand SIMULIA™.
A complete finite element model for heat transfer analysis establishment should contain model inputs characterisation, meshing method selection, geometry, material properties, heat source and boundary conditions application, heat transfer analysis, and post-processing if needed. Therefore, the methods for establishing and developing the model include 5 main steps.
Step 1 is to characterise and determine the geometry and the boundary conditions used in the model, followed by step 2 meshing method and choice of elements. Step 3 is to apply the moving heat source to the model. A moving heat source will need to include the shape, energy input and velocity of the laser beam. Step 4 is to apply the states variable material properties to develop and adjust the model for the powder bed. The states of the material used in the SLM process may experience changes when the temperature increases or decreases, and this state change should be accounted for in the model. Step 5 is multi-layer model establishment, which is a further step to develop the model into a 3D analysis, and simulate the layer by layer manner of the SLM process.
An overall methodology for the SLM process heat transfer modelling is shown in Figure 4-1. The flowchart shows the main working order for the models developed in step 4 and 5.
Figure 4-1 Overall methodology of the heat transfer model